Composition, structure, bonding and thermoelectric properties of "CuT2P3" and "CuT4P3", members of the T(1-x)(CuP3)x series with T being Si and Ge.
Wang, Peng; Ahmadpour, Faraz; Kolodiazhnyi, Taras; Kracher, Alfred; Cranswick, Lachlan M. D.; Mozharivskyj, Yurij; Dalton transactions (Cambridge, England : 2003) 39 (2010) 1105–1112; doi:10.1039/b914555a

data_7030420
_publ_section_title
;
 Composition, structure, bonding and thermoelectric properties of
 &quot;CuT2P3&quot; and &quot;CuT4P3&quot;, members of the T(1-x)(CuP3)x
 series with T being Si and Ge.
;
_journal_issue                   4
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              1105
_journal_page_last               1112
_journal_paper_doi               10.1039/b914555a
_journal_volume                  39
_journal_year                    2010
_chemical_formula_sum            'Cu1.18 Ge3.63 P3.19'
_chemical_formula_weight         437.27
_chemical_name_systematic
;
?
;
_space_group_IT_number           216
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'F -4 2 3'
_symmetry_space_group_name_H-M   'F -4 3 m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            1
_cell_length_a                   5.3934(16)
_cell_length_b                   5.3934(16)
_cell_length_c                   5.3934(16)
_cell_measurement_reflns_used    1108
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      34.00
_cell_measurement_theta_min      6.55
_cell_volume                     156.89(8)
_computing_cell_refinement       X-Area
_computing_data_collection       X-Area
_computing_data_reduction        X-Red32
_computing_publication_material  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'STOE IPDSII'
_diffrn_measurement_method       'omega scan'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0790
_diffrn_reflns_av_sigmaI/netI    0.0218
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_number            1108
_diffrn_reflns_theta_full        33.99
_diffrn_reflns_theta_max         33.99
_diffrn_reflns_theta_min         6.55
_exptl_absorpt_coefficient_mu    21.805
_exptl_absorpt_correction_T_max  0.5780
_exptl_absorpt_correction_T_min  0.2153
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   X-Red
_exptl_crystal_colour            Black
_exptl_crystal_density_diffrn    4.628
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Shard
_exptl_crystal_F_000             198
_exptl_crystal_size_max          0.155
_exptl_crystal_size_mid          0.090
_exptl_crystal_size_min          0.052
_refine_diff_density_max         0.614
_refine_diff_density_min         -0.305
_refine_diff_density_rms         0.073
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.00
_refine_ls_extinction_coef       0.121(12)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.149
_refine_ls_matrix_type           full
_refine_ls_number_parameters     5
_refine_ls_number_reflns         51
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.149
_refine_ls_R_factor_all          0.0104
_refine_ls_R_factor_gt           0.0104
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0000P)^2^+0.2845P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0248
_refine_ls_wR_factor_ref         0.0248
_reflns_number_gt                51
_reflns_number_total             51
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            b914555a.txt
_cod_data_source_block           cuge2p3
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Cubic' changed to 'cubic' according
to
/usr/data/users/saulius/automatic-downloads/retrospective/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from
2011-04-26.

'_exptl_absorpt_correction_type' value 'Empirical'
changed to 'empirical' according to
/usr/data/users/saulius/automatic-downloads/retrospective/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 
;
_cod_original_sg_symbol_H-M      F-43m
_cod_database_code               7030420